Supramolecular Self-Assembly of Zigzag Coordination Polymer Chains: A Fascinating Three-Dimensional Polycatenated Network Featuring an Uneven “Density of Catenations” and a Three-Dimensional Porous Network
Wang, Xin-Long; Qin, Chao; Wang, En-Bo; Xu, Lin; Crystal Growth & Design 6 (2006) 2061–; doi:10.1021/cg0600997

data_4508696
_publ_section_title
;
 Supramolecular Self-Assembly of Zigzag Coordination Polymer
 Chains:&#x2009; A Fascinating Three-Dimensional Polycatenated Network
 Featuring an Uneven &#x201C;Density of Catenations&#x201D; and a
 Three-Dimensional Porous Network
;
_journal_issue                   9
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              2061
_journal_paper_doi               10.1021/cg0600997
_journal_volume                  6
_journal_year                    2006
_chemical_formula_moiety         'C28 H22 Cd N2 O6'
_chemical_formula_sum            'C28 H22 Cd N2 O6'
_chemical_formula_weight         594.88
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 105.51(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.257(2)
_cell_length_b                   18.988(4)
_cell_length_c                   15.296(3)
_cell_measurement_reflns_used    21311
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      3.04
_cell_volume                     2870.6(11)
_computing_cell_refinement       'RAPID AUTO'
_computing_data_collection       'RAPID AUTO'
_computing_data_reduction        'RAPID AUTO'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.973
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Rigaku RAXIS RAPID IP'
_diffrn_measurement_method       Oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Rotation anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0731
_diffrn_reflns_av_sigmaI/netI    0.0570
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            21311
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         3.04
_exptl_absorpt_coefficient_mu    0.801
_exptl_absorpt_correction_T_max  0.8758
_exptl_absorpt_correction_T_min  0.8434
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8 March, 1995'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.377
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1200
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.17
_refine_diff_density_max         0.822
_refine_diff_density_min         -0.624
_refine_diff_density_rms         0.106
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     334
_refine_ls_number_reflns         4922
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.035
_refine_ls_R_factor_all          0.0808
_refine_ls_R_factor_gt           0.0520
_refine_ls_shift/su_max          0.021
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0722P)^2^+2.9345P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1249
_refine_ls_wR_factor_ref         0.1393
_reflns_number_gt                3516
_reflns_number_total             4922
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg0600997sup2.cif
_cod_data_source_block           www
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        2870.5(10)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               4508696